Upload
others
View
13
Download
0
Embed Size (px)
Citation preview
Volume 1, Number 1 (March, 2008) p. 1 - 16 • ISSN 1983-4195
Similarities between punching and shear strength of steel fiber reinforced concrete (SFRC) slabs and beams
Similaridades entre resistência à punção em lajes-cogumelo e ao cisalhamento em vigas de concreto armado com fibras de aço
J.B. DE HANAIa
K.M.A. HOLANDAb
© 2008 IBRACON
a Escola de Engenharia de São Carlos da Universidade de São Paulo, Departamento de Engenharia de Estruturas, e-mail: [email protected], Av. Trabalhador Sao-Carlense, 400, São Carlos – SP, 13566-590, Brasil.
b Conselho Nacional de Desenvolvimento Científico e Tecnológico (CNPq), e-mail:[email protected], SEPN 509, Bloco A, Ed. Nazir I, Brasilia – DF, 70750-501, Brasil.
Abstract
Resumo
This paper discusses the influence of steel fiber in both punching strength of flat slabs and shear strength of concrete beams. Similarities in the structural behavior were observed in an experimental analysis of analogous slabs and beams. The analogous slabs and beams had the same height, longitudinal reinforcement ratio and concrete properties. Concrete mixtures were designed to attain different strength levels, from ordinary to high-strength range. Hooked-end steel fibers with circular section and rectangular section and different aspect ratios were used. Ultimate load capacity and ductility of analogous slabs and beams showed the same performance tendencies as the fiber content varied from 0% to 2%. Analytical investigations were developed to evaluate the ultimate load capacity of slabs and beams. The main conclu-sions are: a) shear tests on prismatic beams provide useful information for steel fiber reinforced concrete (SFRC) mixture design for slab application; b) theoretical strength models that have a linear dependence on fiber content can be used to predict the effect of fiber addition.
Keywords: punching shear; shear strength; flat slab; beam; steel fiber reinforced concrete (SFRC).
O artigo analisa a influência da adição de fibras de aço ao concreto, tanto na resistência à punção em lajes-cogumelo quanto na resis-tência ao cisalhamento em vigas de concreto armado. Pela análise dos resultados de ensaios de modelos estruturais de lajes e vigas em condições análogas, foram identificadas similaridades de efeitos no seu comportamento estrutural. As lajes e vigas análogas testadas tinham a mesma altura, taxa de armadura longitudinal e propriedades do concreto. Os concretos aplicados foram dosados para atingir di-ferentes níveis de resistência, inclusive aquelas consideradas elevadas. As fibras empregadas eram de fios de seção transversal circular e retangular, com ganchos nas extremidades e diferentes relações de aspecto. A capacidade resistente última e a ductilidade das lajes e vigas análogas mostraram as mesmas tendências, conforme o volume de fibras de aço variou entre 0% e 2%. Desenvolveu-se uma análise teórica para avaliar a capacidade resistente última das lajes e vigas, sendo que as principais conclusões foram: a) os ensaios de flexão sobre prismas de concreto fornecem informações muito úteis para a dosagem de concretos com fibras de aço e sua aplicação em lajes sujeitas à punção; b) modelos teóricos que assumem uma dependência linear entre capacidade resistente (à punção e ao cisalha-mento) e o volume de fibras oferecem resultados satisfatórios para dimensionamento.
Palavras-chave: concreto com fibras; laje-cogumelo; vigas; punção; cisalhamento.
2 IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
Similarities between punching and shear strength of steel fiber reinforced concrete (SFRC) slabs and beams
1. Introduction
1.1 Brief review
Flat slab structural systems have widely been used in building con-struction due to several advantages that include architectural de-sign and fast construction methods. Technological advances in this field came with new prestressing materials and techniques, also the application of special concretes such as the self-compacting concrete and high-strength concrete.Punching shear strength of flat slabs is the most important limita-tion of this particular structural system due to its fragile nature. This kind of failure must be avoided by providing the slab-column con-nection of efficient mechanisms of strength and ductility.Several investigations have shown the performance improvement of the slab-column connection by using steel fiber concrete. Both strength and ductility enhancement were observed by Swamy & Ali [1], Alexander & Simmonds [2], Theodorakopoulos & Swamy [3],
Tan & Paramasivam [4], Shaaban & Gesund [5], Harajli et al. [6], Hughes & Xiao [7], Prisco & Felicetti [8] and McHarg et al. [9].The combination of high-strength concrete and steel fibers shows interesting results because punching strength can be raised without loss in ductility. Zambrana Vargas [10], Azevedo [11] and Holanda [12] performed punching tests in many combinations of ordinary and high strength concrete, steel fibers and shear reinforcement. The test results confirmed the expectations, also revealing a good efficiency of steel fibers in high-strength matrices.It is well known that phenomena of punching in slabs and shear in beams can be represented by strength mechanisms of the same na-ture. In both cases the ultimate load is affected by the intensity of diago-nal tension, arching effect, friction action in cracks and dowel action.A tentative analysis of the similarities between punching strength in slabs and shear strength in beams is reported in this paper. Slab-column connections and analogous simply supported beams were tested, mainly to observe the effect of steel fiber addition to con-crete on the ultimate load and ductility. The variables in the tests were concrete strength, type and volume fraction of steel fibers,
3IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
J.B. DE HANAI | K.M.A. HOLANDA
2. Materials and experimental program
Five series of analogous slabs and beams (S1 to S5) were tested.In Series 1, concrete compressive strength was kept around 25 MPa and steel fiber volume fraction was considered equal to 0%, 1% and 2%.In Series 2 and 3, concrete strength was about 56 MPa and steel fi-ber volume fraction varied in the same way. In Series 3, only beams with 170 mm height were tested, to observe any size effect.In Series 4 punching test results were taken from Azevedo [11] in which a different type of steel fiber was used (0%, 0.75% and 1.5% volume fraction). Complementary slabs and beams were tested to complete the series and concrete strength was kept around 40 MPa.Finally, in Series 5 only beams were tested to complement the test results obtained by Zambrana Vargas [10]. Concrete strength was about 73 MPa and a third type of steel fiber (0%, 0.75% and 1.5% volume fraction) was added.
2.1 Materials
Concrete mixtures were designed to attain different strength lev-els, from ordinary to high-strength range. ASTM Type IS Portland cement (blended blast furnace slag cement), river sand (fineness modulus equal to 2.37), basalt coarse aggregate (maximum size equal to 6.3 mm) and a superplasticizer admixture were used in concrete mixtures for test series S1 to S4. For the series S5, ASTM Type III Portland cement (high early strength cement) and silica fume were also applied. Hooked-end steel fibers with circular sec-tion and rectangular section and different aspect ratios were used. Table 1 summarizes the concrete mixtures composition.
height of slabs and beams and dimension of the loaded area.The ACI 318M-02 [13] design method was adapted to consider the steel fiber action. The theoretical results are compared to the experimental ones and a final discussion is presented.
1.2 Justification
Slabs and beams without transversal reinforcement may reach an ultimate limit state without yielding of the flexural reinforcement. A fragile failure may occur and this kind of ruin must be avoided.Strength mechanisms in slab punching and beam shear are sim-ilar, both in relation to the main mechanisms (diagonal tension, contribution of the compressed struts) and to complementary mechanisms (dowel effect of the longitudinal reinforcement, friction between crack surfaces, arching effect, strut flexural stiffness).The rising of concrete strength increases the punching strength and shear strength, but high-strength concrete presents lower toughness. When fracture occurs, its surface is smoother and this leads to decreasing of the positive effects of friction and interlock-ing of aggregates. The addition of steel fibers affords higher tough-ness to concrete and provides bridging effects across cracks, both in the fracture surface and around the reinforcement.The test results of this research showed the feasibility of shear tests on prismatic beams to choose the type and amount of steel fibers to be used in flat-slabs. These tests would be simpler and cheaper than the complex slab-column connection tests.There are several theoretical approaches that explain the shear transfer in a slab-internal column connection, with or without punch-ing reinforcement. However, none of the design codes considers fiber’s contribution in punching strength of flat slabs.
4 IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
Similarities between punching and shear strength of steel fiber reinforced concrete (SFRC) slabs and beams
2.2 Punching Tests on Slabs
In Series 1, 2 and 4 punching tests were carried out on 1160 mm square and 100 mm thickness slabs. All the slabs were supported along their perimeter and tested by pushing down on the center of the slab through a hydraulic actuator. This means that, referring to a real situation in a building, the load was applied upside down on the tests. Figure 1 illustrate the loading test system.Figures 2 and 3 show the slab reinforcement characteristics. The drawings show the reinforcing bars as they were positioned for slab casting, in the same way that occurs in a real situation. The top flexural reinforcement consisted of 10 mm diameter bars, 17 in one direction (effective depth of 85 mm) and 20 in the other (effective depth of 75 mm), in order to obtain the same resistant moment in both directions. The bottom flexural reinforcement consisted of nine 5 mm diameter bars in each direction. Some steel reinforcement bars were instrumented with electrical strain gages to monitor the strains and forces during the tests and to better evaluate the structural behavior of the slabs. Figure 4 shows the location of the strain gages and displacement transducers.The test force was introduced by a servo-hydraulic actuator over a square steel plate (80 mm side), in a 0.005 mm/s displacement-controlled mode.
2.3 Shear Tests on Beams
In series 1, 2 and 4 shear tests were carried out on 600 mm length, 100 mm height and 120 mm width beams. The height and the flex-ural reinforcement ratio of these beams were the same of the analo-gous slabs. The beams were simply supported at their ends and tested by pushing down on the center through a hydraulic actuator.The beams bottom flexural reinforcement of Series 1, 2 and 4 consisted of two 10 mm diameter bars (effective depth of 85 mm) and the top flexural reinforcement consisted of two 5 mm diameter bars. Also in the beams some steel reinforcement bars were in-strumented with electrical strain gages to monitor the strains and forces during the tests. Figure 5 shows the reinforcement and in-strumentation details for these series.
In Series 3 the beam’s height was enlarged to 170 mm to observe eventual size effect in the search of similarities amongst beams and slabs. The beam’s length was 1100 mm and the beam’s width was 130 mm. The flexural reinforcement ratio was maintained.In Series 5 the width of the beams was reduced to 110 mm to adjust the flexural reinforcement ratio to be the same of the main reinforcement of the slabs tested by Zambrana Vargas [10]. The beams bottom flexural reinforcement of Series 5 consisted of four 10 mm diameter bars (effective depth of 155 mm) and the top flex-ural reinforcement consisted of two 5 mm diameter bars.Table 2 summarizes the main characteristics of the experimental program.
3. Experimental results and discussions
Table 3 presents the ultimate load values recorded on the test of slabs and beams performed by Holanda [12] and Table 4 presents test data from Azevedo [11] and Zambrana Vargas [10].The graphic in Figure 6 shows a relation between the concrete tensile strength (normalized by the square root of the concrete compressive strength) with the fiber volume fraction added to con-crete slabs. The relation showed to be almost linear. Since con-crete strength varied on each test series, normalization was ap-plied to reduce the influence of the concrete tensile strength on the test result analysis. Square root of concrete compressive strength was used because it better represents the tensile strength than the plain compressive strength.All slabs were designed to fail by punching shear, what really hap-pened. In the steel fiber reinforced slabs, there was a tendency of ultimate loads to be closer to the estimated load for flexural failure, as more fibers were added to concrete. This means that the ad-dition of steel fibers contributed to the ductility of the connection in the rupture. From the test results, it can be seen that the best performance both in strength and ductility was obtained in Series 2, using high strength concrete and 2% of steel fibers.In all test series, both in slabs and beams, it was observed that strength and ductility increased as the volume of steel fibers in-creased (Figures 7 and 8). Load-deflection diagrams observed
5IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
J.B. DE HANAI | K.M.A. HOLANDA
6 IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
Similarities between punching and shear strength of steel fiber reinforced concrete (SFRC) slabs and beams
in slabs and beams were similar, mainly looking at the variation of fibers volume. Therefore, a previous performance analysis of beams may offer useful data to design the type and amount of fibers to be used in slabs. The main advantage of this approach is that several small beams can be tested at low cost and, with help of Fracture Mechanics methods, a confident design of fiber reinforced concrete can be designed for slab punching strength and ductility.The largest normalized punching strength of slabs without fibers was observed in Series 1 slabs (fc14 ≅ 25 MPa), followed by Series 4 slabs (fc14 ≅ 40 MPa), and at last by Series 2 slabs (fc14 ≅ 60 MPa), due to the brittleness of high strength concrete. By adding fibers, one can notice an inversion of this order for amounts higher than 1.5%. The largest punching strength was obtained in Series 2 slabs, followed by Series 4 slabs and by Series 1 slabs. Fibers were more efficient in the high-strength concrete.In Series 4, the conclusion is that fiber RC 65/30 BN (aspect ratio 66.7) produced greater ductility in slabs than fiber RL 45/50 BN (aspect ratio 48). The modification of the aspect ratio had little influ-ence in the strength of structural elements (Figure 9).Beams without fibers presented a sudden failure by shear after the formation of inclined cracks, as illustrated in Figure 10. The beams reinforced with high ratios of fibers (Figure 11) had a shear failure concurrently with the yielding of flexural reinforcement.As occurred with slabs, steel fiber reinforced beams showed a more ductile failure, with a higher stress level in the flexural re-inforcement, also showing cracks at the maximum bending mo-ment region.In all beams of Series 1 to 4, the failure occurred by fiber pull-out, while in the Series 5 beams fiber rupture occurred. The fibers used in Series 5 did not provide high flexural toughness level.
Many authors mentioned the linear relationship between punching strength and specific fiber volume, at least in an interval of fiber volume fraction between 0 and 2%. This fact was also confirmed by Brazilian researchers. Holanda [12] demonstrates that there is a linear relation in the study of shear in beams. Figures 12 to 14 show diagrams of normalized ultimate load versus fiber volume fraction for specimens of Series 2 to 5. Normalization was made dividing the ultimate loads by the square root of the concrete compressive strength, to reduce the influence of concrete strength variation.Figure 15 shows graphics of relative load (load divided by ultimate load) versus relative displacement (displacement divided by ulti-mate displacement) of slabs and beams, with the same concrete strength and the same amount of fibers. It is noticed that in both graphics, the pre-peak section of the slab and of both beams is almost coincident.
4. Analytical investigation
4.1 Analysis of beams according to ACI 318M-02
The ACI 318M-02 [13] adopts a relation between concrete ten-sile strength (split test) and the square root of the compressive strength, as shown in Equation 1.
7IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
J.B. DE HANAI | K.M.A. HOLANDA
being fc the concrete strength to axial compression and fsp the concrete tensile strength (split test), both in MPa.Many authors demonstrate a strong correlation between shear strength and the square root of concrete compressive strength. This corresponds to an indirect correlation of shear strength to the concrete tensile strength.It is well known that when a low volume fraction of steel fibers are added to concrete, the first cracking strength is not significantly
increased. However, ductility and post-cracking resistance can be increased, thus providing shear resistance by bridging di-agonal cracks. In addition, because fibers would control the opening of these cracks, shear resistance through aggregate interlock would likely be increased.Equation 1 from ACI Code is very simple and affordable for practical calculations. Therefore, a tentative analysis was done to verify if it also is able to represent by means of a
8 IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
Similarities between punching and shear strength of steel fiber reinforced concrete (SFRC) slabs and beams
single parameter, the tensile strength of fiber reinforced con-crete, the shear load capacity increase in situations of diago-nal tension rupture.
At first, to correlate the concrete tensile strength to the com-pressive strength of the steel fiber reinforced concrete, a lin-ear regression of experimental results was made. Equation
9IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
J.B. DE HANAI | K.M.A. HOLANDA
2 express this relationship in a similar format of Equation 1.
being fsp, fc given in MPa and Vf in %.The ACI 318M-02 [13] prescribes Equation 3 to evaluate the ulti-mate shear force for beams without stirrups:
where:fc: concrete axial compressive strength;d: effective slab depth;b: beam length;
10 IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
Similarities between punching and shear strength of steel fiber reinforced concrete (SFRC) slabs and beams
11IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
J.B. DE HANAI | K.M.A. HOLANDA
being fc given in MPa; and b and d in cm.To consider the steel fiber effect, a certain way the value of fsp obtained from Equation 2 can be introduced in Equation 3, thus a modified equation from ACI 318M-02 [13] can be stated (Equation 4). Some adaptations were done to preserve the ad-justment and safety factors that are implicit in the coefficient 0.166 of Equation 3.
being fc given in MPa; b, d in cm and Vf in %.Theoretical values obtained by using Equation 4 showed rea-sonable correlation with the beam test results, as demonstrat-ed in Figure 16. It can be seen that the tested equation repre-sents the experimental tendencies, since the linear regression results in an almost parallel line to the Vf axis and on the safe side, as general.
4.2 Analysis of slabs according to ACI 318M-02
For the analysis of the slab tests, another relationship between SFRC tensile strength and compressive strength was found for the
12 IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
Similarities between punching and shear strength of steel fiber reinforced concrete (SFRC) slabs and beams
test results. Equation 5 express this correlation, in a similar format of Equation 2.
being fsp and fc given in MPa and Vf in %.The ACI 318M-02 [13] prescribes Equation 6 to evaluate the ul-timate punching load for slabs without transversal reinforcement and square section columns.
where:fc: concrete axial compressive strength;bo = 4(c+d) → perimeter where punching occurs;d: effective slab depth;c: column length;being fc given in MPa; and bo, d in cm.
13IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
J.B. DE HANAI | K.M.A. HOLANDA
14 IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
Similarities between punching and shear strength of steel fiber reinforced concrete (SFRC) slabs and beams
Alike in case of beams, the value of fsp (from Equation 5) is intro-duced in Equation 6 to consider the effect of steel fibers in punching strength. Adaptations were done to preserve the adjustment and safety factors that are implicit in the coefficient 0.3321 of Equation 6. By this procedure Equation 7 was obtained.
being fc given in MPa; bo, d in cm and Vf in %.Figure 17 shows an evaluation of the response of Equation 7 when compared to the experimental data obtained in this research, together with some of Zambrana Vargas [10] and Azevedo [11]. It can be seen that Equation 7 offers a reasonable response to the experimental ten-dencies, as the fiber volume increases. However, since the linear trend is not parallel to the Vf axis, an additional adjustment must be done. Considering the particular data of this research, an empirical coefficient of about 0.3102 was applied to reduce the effect of Vf in Equation 7. This procedure leads to Equation 8, here called ACI 318 Modified Equation. The performance of Equation 8 is also shown in Figure 18.
5. Conclusions
Based on the experimental results, it can be concluded that there are unequivocal similarities between punching shear strength in flat slabs and shear strength in analogous beams. The analogous slabs and beams must have the same height, longitudinal rein-forcement ratio and concrete properties. Therefore, shear tests on small prismatic beams can be performed to get useful indicators for the steel fiber reinforced concrete mixture design, looking at its application in flat slab-column connections.In addition to load capacity information, the analysis of these similar-ities can give information about ductility of the connection, as shown in load versus deflection diagrams of analogous slabs and beams.In this experimental program only three types of fibers were used, since it aimed at evaluating other parameters, such as concrete strength, fiber volume, effective depth and column side length.ACI Code gives very simple equations to estimate shear strength of beams and punching strength of slabs. In these equations, the square root of concrete compressive strength corresponds to an in-direct correlation of shear strength to the concrete tensile strength.Theoretical analysis based on ACI Modified Equations, adapted to steel fiber reinforced concrete, both for slabs and for beams, pro-vided good indicators of shear strength of beams without stirrups and punching shear strength of slabs without transversal reinforce-ment. Test results also showed that theoretical strength models, based on linear dependence on fiber content, can be used to pre-dict the effect of fiber addition.
15IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
J.B. DE HANAI | K.M.A. HOLANDA
Future research works in this way can lead to good knowl-edge improvements, by detailing other aspects such as the application of other kinds of fibers, with different aspect ra-tios; the test of analogous slabs and beams of larger di-mensions, to check the scale effect; the extension of the experimental study to slabs and beams with transversal re-inforcement; and the variation of the flexural reinforcement ratio in the test series.
6. Acknowledgements
The authors thankfully acknowledge the financial support of CNPq – National Council for Scientific and Technological Development and FAPESP –State of Sao Paulo Research Foundation, also to Belgo Mineira Bekaert Arames S/A, Holdercim Brasil S/A and Je-ruel Artefatos Plasticos Ltda., for supplying the materials used in the research.
16 IBRACON Structures and Materials Journal • 2008 • vol. 1 • nº 1
Similarities between punching and shear strength of steel fiber reinforced concrete (SFRC) slabs and beams
7. References
[01] Swamy R.N., Ali S.A.R. Punching shear behavior of reinforced slab-column connections made with steel fiber concrete. Journal of the American Concrete Institute 1982;79(5):392-406. [02] Alexander S.D.B., Simmonds S.H. Punching shear tests of concrete slabs-column joints containing fiber reinforcement. ACI Structural Journal 1992;89(4):425-432. [03] Theodorakopoulos D.D., Swamy N. Contributions of steel fibers to the strength characteristics of lightweight concrete slab-column connections failing in punching shear. ACI Structural Journal 1993;90(4):342-355. [04] Tan K.H., Paramasivam P. Punching shear strength of steel fiber reinforced concrete slabs. Journal of Materials in Civil Engineering 1994;6(2):240-253. [05] Shaaban A.M., Gesund H. Punching shear strength of steel fiber reinforced concrete flat plates. ACI Structural Journal 1994;91(4):406-414. [06] Harajli M.H., Maalouf D., Khatib H. Effect of fibers on the punching shear strength of slab-column connections. Cement & Concrete Composites 1995;17(2):161-170. [07] Hughes B.P., Xiao Y. Flat slabs with fibre or link reinforcement at slab-column connections. Institution of Civil Engineers Structures & Buildings 1995;110:308-321. [08] Prisco M., Felicetti R. Some results on punching shear in plain and fibre-reinforced micro-concrete slabs. Magazine of Concrete Research 1997;49(180):201-219. [09] McHarg P.J., Cook, W.D., Mitchell D., Yoon Y.S. Benefits of concentrated slab reinforcement and steel fibers on performance of slab-column connections. ACI Structural Journal 2000;97 (2):225-234. [10] Zambrana Vargas E.N. Punching shear strength of high strength concrete flat slabs with steel fibers. MSc dissertation. University of Sao Paulo at Sao Carlos, 1997 (in Portuguese). [11] Azevedo A.P. Resistance and ductility of slab-column connections on high strength concrete flat slabs with steel fibers and shear reinforcement. MSc dissertation. University of Sao Paulo at Sao Carlos, 1999 (in Portuguese). [12] Holanda K.M.A. Analysis of strength mechanisms and similarities between punching shear in flat slabs and shear in beams made of steel fiber reinforced concrete. PhD thesis. University of Sao Paulo at Sao Carlos, 2002 (in Portuguese). [13] ACI 318M-02. Building code requirements for structural concrete. American Concrete Institute, Farmington Hills, Michigan, 2002.